Synthesis of novel cone-shaped CaAl-LDH directly on aluminum alloy by a facile urea hydrolysis method
- 144 Downloads
The urea method is one of the unique approaches to synthesize highly crystalline-layered double hydroxides (LDHs). Herein, we synthesized calcium-based layered double hydroxide (CaAl–LDH) directly on Al AA6082 substrate by using the urea hydrolysis reaction, in an effort to obtain highly potential novel cone-shaped unique LDH structure. The as-prepared CaAl-LDH thin film is characterized by X-ray diffraction, Fourier transform spectroscopy, scanning electron microscopy, transmission electron microscopy and further investigated the thermal properties and electron impedance spectra behavior. That simple in situ synthetic approach will be helpful to design environmentally friendly CaAl-LDH thin films that can be further investigated for numerous potential applications like environmental science, catalysts and biomedical applications.
KeywordsUrea hydrolysis Cone-shaped CaAl-LDH thin film In situ growth
Layered double hydroxides (LDHs), considered as ordered layered materials, have been widely investigated in different research fields, for instance, drug delivery system , protective coatings [2, 3], environmental sciences , adsorption [5, 6] and as catalysts , due to their compositional versatility, wide range of structural availability and flexible choice of compositional cations and anions. Layered double hydroxide is represented by a general expression [M1−x2+Mx3+·x(OH)2]Ax/nn−·mH2O] and consists of positively charged layers of mixed metal hydroxides, where some of the divalent (M2) cations are substituted with trivalent (M3) cations, while the net positive charge is compensated through anions (An) intercalations, and results in the formation of brucite-like structure . Generally, two different approaches are employed to synthesize layered double hydroxide system, i.e., co-precipitated  and in situ growth method . The conventional hydrothermal approaches lead to the formation of either hexagonal platelet structure or sand-rose surface morphology. In our recent work, we developed different LDH surface morphologies, for instance, cauliflower, stone-like structure, with the variation of synthetic parameters . Dutta et al. designed the hydrophobic cone-shaped structure modified by dodecyl sulfate ions to enhance the absorption capacity of CaAl-LDH through the co-precipitation method . Recently, we investigated CaAl-LDH, exhibiting various surface morphologies, grown directly on an aluminum substrate to investigate the corrosion resistance properties . It has been reported that well-crystallized, highly active LDH can also be synthesized by urea hydrolysis method and can be considered as an efficient approach to design a highly oriented LDH structure [12, 13]. In the present study, novel cone-shaped CaAl-LDH is synthesized on the aluminum substrate by single-step urea hydrolysis method. Urea is found to impart some excellent features in the formation of LDH and can be helpful to modify the textural properties, often resulting in the mono-dispersed particle distribution and uniform precipitation due to the hydrolysis of urea upon the thermal treatment . From the last few years, LDH structure ranging from the nanosize spheres and platelet structures to LDH belts are formed to utilize it in various applications. This study is the example of a single-step facile formation of cone-shaped, well-ordered CaAl-LDH grown directly on aluminum substrate. The major advantages of CaAl-LDH formed by urea hydrolysis method are as follows: (1) single-step in situ cone-shaped LDH synthetic route, (2) wel- ordered, morphological alteration along with homogenous particles for numerous applications in the fields of nanomaterial’s and composites and (3) cone-shaped LDH particles with preferential growth perpendicular to the substrate, with crystallite size distribution much narrower than conventional co-precipitation methods.
2 Synthesis of nanocones CaAl-LDH
The cone-shaped CaAl-LDH thin film was grown through the urea hydrolysis approach. In general, the aluminum specimen (3.14 cm2) was initially ground from 500 to 1000, 2400 grit SiC paper, respectively, and was washed with deionized water and further was treated ultrasonically in pure ethanol for 10 min. Finally, the specimens were etched by using 0.1 M NaOH solution for 1 min. The pretreated aluminum substrate actually acts as the source of Al+3 which provides a building block for the synthesis of LDH on it. 0.03 M CaNO3·4H2O and 0.18 M urea (1:1) were prepared and were transferred into 100 mL Teflon-lined autoclave, while the pretreated aluminum substrates (3.14 cm2) were placed in the prepared solution and were treated in an oven at 120 °C for 18 h. The initial pH of the prepared solution was 5.36, which on completion of the experiment approached 9.7.
The nanocone-shaped CaAl-LDH thin-film structure was confirmed by the scanning electron microscopy (JEOL JSM-6330F) and transmission electron microscopy (FEI Talos F200X). The X-ray diffractometer (Bruker D5005, λ = 1.5406 Å−1) was used to characterize the crystal structure. The surface functional groups of the film were recorded by FTIR (NICOLET MAGNA 560) in ATR mode. The TGA analysis of CaAl-LDH was obtained by using TA instruments [TGA Q5000 IR thermobalance (New Castle, DE, USA)] with a sample size of 7 mg (scraped from the coated specimen) at a heating rate of 10 °C/min under air flow (10 mL/min), while DSC analysis was studied through Mettler DSC30 calorimeter (Columbus, OH, USA), using 10 mg CaAl-LDH powder under an air flow of 10 mL/min up to 600 °C temperature. EIS measurements were acquired by using PAR (Parstat 2273 equipment) for a frequency range of 100 kHz–10 mHz, with an amplitude perturbation of 5 mV (rms). The measurement was performed in 0.1 M NaCl solution at ambient conditions.
4 Results and discussion
The “001” reflection peak at 2(θ) of 12.29° indicated a basal spacing of 0.72 nm. The resultant basal spacing is specific for the family of LDHs, where positively charged layers interlayer anions hold the OH− . Here, the basal spacing did not correlate with the traditional NO3−1 spacing, possibly due to the following reasons: (1) the anions intercalation varies in terms of orientations, for instance, nitrate anions can intercalate in three specific orientations from “flatter” to “stacked” orientation. Among them, flatter orientation can show a reduction in basal spacing , (2) the water molecules are trapped inside the interlayers along with anions in various fashions, which affect the d-spacing. (3) Nitrate anions can be absorbed on the diffuse electrical layers of LDH. Further, the formation of tricalcium aluminate (TCA) may cause the suppression of nitrates inside the interlayer’s [16, 19]. However, FTIR analysis has shown the characteristics peak of NO31− groups and confirmed the presence of nitrate groups in the LDH system. It seems that TCA formation caused suppression of nitrate intercalation and nitrate groups adsorbed on the diffused electrical layers.
The co-precipitated CaAl-LDH powders are actively investigated as catalysts, biomedical applications and so on [25, 26]. The advantages of novel cone-shaped CaAl-LDH films grown on the metallic substrate will be helpful for the design of potentially active LDH for above-said applications, owing to the unique structure, preferential growth and geometry due to the activated structure. In a nutshell, this work gives an insight on the in situ grown cone-shaped CaAl–NO3–LDH structure, and the geometry capable to modify further with inorganic and organic ions due to low ion exchange equilibrium constant of interlayer NO3−1 anions.
In summary, we describe the development of cone-shaped CaAl–NO3–LDH on AA6082 using the urea hydrolysis method. The XRD and FTIR analysis confirmed the formation of CaAl-LDH on the aluminum surface, while microscopic studies have shown a well-ordered cone-like LDH structure. From TGA results, around 40% of mass losses were observed through the thermal decomposition along with significant impedance response in EIS analysis. In summary, this research provides an insight on the direct synthesis of cone-shaped CaAl–NO3–LDH on the aluminum surface and provides a view on the structural investigation of well-ordered, cone-shaped, uniform homogeneous LDH structure. These features would support our knowledge of control environmental friendly CaAl-LDH thin film, resultant properties and possible applications.
Compliance with ethical standards
Conflict of interest
The authors declare no conflict of interest.
- 17.Rousselot I, Taviot-Guého C, Leroux F, Léone P, Palvadeau P, Besse JP (2002) Insights on the structural chemistry of hydrocalumite and hydrotalcite-like materials: investigation of the series Ca2M3+(OH)6Cl· 2H2O (M3+: Al3+, Ga3+, Fe3+, and Sc3+) by X-ray powder diffraction. J Solid State Chem 167(1):137–144CrossRefGoogle Scholar
- 23.Ni ZM, Xia SJ, Fang CP, Wang LG, Hu J (2008) Synthesis, characterization and thermal property of Cu/Co/Mg/Al hydrotalcite like compounds. Rare Metal Mater. Eng 37:634–637Google Scholar